# Electronic Supplementary Material (ESI) for Journal of Materials Chemistry C.
# This journal is © The Royal Society of Chemistry 2020

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_a
_database_code_depnum_ccdc_archive 'CCDC 1900321'
loop_
_audit_author_name
_audit_author_address
'Anyi Zhou'
;Fujian Institute of Research on the Structure of Matter
China
;

_audit_update_record             
;
2019-02-28 deposited with the CCDC.	2020-04-28 downloaded from the CCDC.
;
_audit_creation_date             2019-02-15
_audit_creation_method           
;
Olex2 1.2
(compiled 2017.08.10 svn.r3458 for OlexSys, GUI svn.r5381)
;
_chemical_name_common            ?
_chemical_name_systematic        
;
 ? 
;
_chemical_formula_moiety         '0.5(Ba12 In12 Se38 Zn8)'
_chemical_formula_sum            'Ba6 In6 Se19 Zn4'
_chemical_formula_weight         3274.68
_chemical_absolute_configuration ad
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Ba Ba -0.3244 2.2819 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
In In -0.7276 1.3100 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Se Se -0.0929 2.2259 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Zn Zn 0.2839 1.4301 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      tetragonal
_space_group_IT_number           113
_space_group_name_H-M_alt        'P -4 21 m'
_space_group_name_Hall           'P -4 2ab'
loop_
_space_group_symop_id
_space_group_symop_operation_xyz
1 'x, y, z'
2 'y, -x, -z'
3 '-x, -y, z'
4 '-y, x, -z'
5 'x+1/2, -y+1/2, -z'
6 '-y+1/2, -x+1/2, z'
7 '-x+1/2, y+1/2, -z'
8 'y+1/2, x+1/2, z'

_cell_length_a                   17.3486(14)
_cell_length_b                   17.3486(14)
_cell_length_c                   6.7184(8)
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_volume                     2022.1(3)
_cell_formula_units_Z            2
_cell_measurement_reflns_used    7433
_cell_measurement_temperature    293.1500
_cell_measurement_theta_max      27.4894
_cell_measurement_theta_min      2.6253
_exptl_absorpt_coefficient_mu    28.507
_exptl_absorpt_correction_T_max  1.0000
_exptl_absorpt_correction_T_min  0.5125
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   ?
_exptl_crystal_colour            red
_exptl_crystal_density_diffrn    5.378
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       Prism
_exptl_crystal_F_000             2792
_exptl_crystal_size_max          0.2
_exptl_crystal_size_mid          0.1
_exptl_crystal_size_min          0.1
_exptl_special_details           
;
 ?
;
_diffrn_reflns_av_R_equivalents  0.0642
_diffrn_reflns_av_unetI/netI     0.0404
_diffrn_reflns_limit_h_max       22
_diffrn_reflns_limit_h_min       -22
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_k_min       -22
_diffrn_reflns_limit_l_max       8
_diffrn_reflns_limit_l_min       -8
_diffrn_reflns_number            17366
_diffrn_reflns_theta_full        27.49
_diffrn_reflns_theta_max         27.49
_diffrn_reflns_theta_min         2.63
_diffrn_ambient_temperature      293.1500
_diffrn_detector_area_resol_mean 28.5714
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_details      
;
scan:
	Number of images: 360
	           Slice: -115.0000 - 65.0000
	     Image width: 0.5000
	        Exp time: 5.0000
	   Rotation axis: Omega
	           Omega: 0.0000
	             Chi: 45.0000
	             Phi: 0.0000
	             XTD: 45.0793
	          2theta: -24.8100
scan:
	Number of images: 280
	           Slice: -115.0000 - 25.0000
	     Image width: 0.5000
	        Exp time: 5.0000
	   Rotation axis: Omega
	           Omega: 0.0000
	             Chi: 45.0000
	             Phi: 90.0000
	             XTD: 45.0793
	          2theta: -24.8100
scan:
	Number of images: 160
	           Slice: -115.0000 - -35.0000
	     Image width: 0.5000
	        Exp time: 5.0000
	   Rotation axis: Omega
	           Omega: 0.0000
	             Chi: 45.0000
	             Phi: 180.0000
	             XTD: 45.0793
	          2theta: -24.8100
;
_diffrn_measurement_device       
;
Saturn724+ (2x2 bin mode)
;
_diffrn_measurement_device_details 
;
AFC10: Fixed Chi 2 circle
;
_diffrn_measurement_device_type  'Mercury70 (2x2 bin mode)'
_diffrn_measurement_method       CCD_Profile_fitting
_diffrn_number_total             2528
_diffrn_orient_matrix_type       d*Trek
_diffrn_orient_matrix_UB_11      -0.0164
_diffrn_orient_matrix_UB_12      0.0517
_diffrn_orient_matrix_UB_13      0.0194
_diffrn_orient_matrix_UB_21      0.0309
_diffrn_orient_matrix_UB_22      0.0254
_diffrn_orient_matrix_UB_23      -0.0415
_diffrn_orient_matrix_UB_31      -0.1183
_diffrn_orient_matrix_UB_32      -0.0035
_diffrn_orient_matrix_UB_33      -0.0903
_diffrn_radiation_detector       CCD
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   'Sealed Tube'
_diffrn_source_current           80.0000
_diffrn_source_power             4.0000
_diffrn_source_voltage           50.0000
_diffrn_special_details          
;
 ?
;
_diffrn_standards_decay_%        ?
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_number         ?
_reflns_number_gt                2404
_reflns_number_total             2433
_reflns_threshold_expression     >2sigma(I)
_computing_cell_refinement       'CrystalClear (Rigaku Inc., 2008)'
_computing_data_collection       'CrystalClear (Rigaku Inc., 2008)'
_computing_data_reduction        'CrystalClear (Rigaku Inc., 2008)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'XL (Sheldrick, 2008)'
_computing_structure_solution    'XS (Sheldrick, 2008)'
_refine_diff_density_max         1.647
_refine_diff_density_min         -2.029
_refine_diff_density_rms         0.246
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.00(3)
_refine_ls_extinction_coef       0.00153(7)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.149
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     101
_refine_ls_number_reflns         2433
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0324
_refine_ls_R_factor_gt           0.0317
_refine_ls_restrained_S_all      1.149
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0190P)²+26.8330P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0730
_refine_ls_wR_factor_ref         0.0734
_refine_special_details          
;
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
;
_olex2_refinement_description    
;
1. Twinned data refinement
 Scales: 0.92(2)
 0.08(2)
2. Uiso/Uaniso restraints and constraints
Uanis(In5) = Uanis(Zn5)
Uanis(In4) = Uanis(Zn4)
Uanis(In3) = Uanis(Zn3)
3. Others
 Fixed Sof: In3(0.5) Zn3(0.5) In4(0.25) Zn4(0.25) In5(0.25) Zn5(0.25)
;
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_calc_flag
_atom_site_disorder_assembly
_atom_site_disorder_group
_atom_site_site_symmetry_order
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
Ba1 Ba -0.49224(4) -0.27329(4) 0.46074(10) 0.02162(17) Uani 1 d . . 1 . . .
Ba0A Ba -0.13671(4) -0.36329(4) 0.08568(14) 0.0192(2) Uani 1 d . . 2 S T P
In3 In -0.3609(17) -0.3166(17) -0.050(4) 0.0178(3) Uani 0.50 d . 1 1 . . .
Zn3 Zn -0.361(3) -0.317(3) -0.048(7) 0.0178(3) Uani 0.50 d . 2 1 . . .
In4 In -0.3994(8) -0.1006(8) 0.0682(16) 0.0112(12) Uani 0.50 d . 1 2 S T P
Zn4 Zn -0.3976(13) -0.1024(13) 0.100(3) 0.0112(12) Uani 0.50 d . 2 2 S T P
In5 In -0.2718(12) -0.2282(12) -0.558(2) 0.0274(17) Uani 0.50 d . 1 2 S T P
Zn5 Zn -0.272(2) -0.228(2) -0.589(5) 0.0274(17) Uani 0.50 d . 2 2 S T P
Se1 Se -0.5000 0.0000 -0.0571(3) 0.0167(4) Uani 1 d . . 4 S T P
Se2 Se -0.37544(6) -0.12456(6) -0.5483(3) 0.0173(3) Uani 1 d . . 2 S T P
Se3 Se -0.32020(6) -0.34958(6) -0.70464(17) 0.0186(2) Uani 1 d . . 1 . . .
Se4 Se -0.24049(7) -0.25951(7) -0.2169(2) 0.0206(3) Uani 1 d . . 2 S T P
Se5 Se -0.46907(6) -0.21963(6) -0.04046(18) 0.0196(2) Uani 1 d . . 1 . . .
Se6 Se -0.41962(7) -0.42146(6) -0.25276(16) 0.0190(2) Uani 1 d . . 1 . . .
Se7 Se -0.59921(6) -0.09921(6) -0.5651(2) 0.0168(3) Uani 1 d . . 2 S T P
In1 In -0.5000 0.0000 -0.4614(3) 0.0475(6) Uani 1 d . . 4 S T P
In2 In -0.5000 -0.5000 0.0000 0.0196(3) Uani 1 d . . 4 S T P


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ba1 Ba0A 4.6023(10) 4_456 ?
Ba1 In3 4.07(3) 1_556 ?
Ba1 In5 3.906(16) 1_556 ?
Ba1 Zn5 3.92(3) 1_556 ?
Ba1 Se2 3.2814(7) 1_556 ?
Ba1 Se3 3.2981(13) 4_455 ?
Ba1 Se3 3.4490(13) 1_556 ?
Ba1 Se5 3.5166(15) . ?
Ba1 Se5 3.5012(15) 1_556 ?
Ba1 Se6 3.2617(13) 4_455 ?
Ba1 Se6 3.4497(13) 1_556 ?
Ba1 Se7 3.5487(8) 1_556 ?
Ba0A In3 4.08(3) 6_445 ?
Ba0A In3 4.08(3) . ?
Ba0A In5 4.09(3) 1_556 ?
Ba0A Zn5 3.97(4) 1_556 ?
Ba0A Se1 3.3596(10) 2_545 ?
Ba0A Se3 3.4891(14) 1_556 ?
Ba0A Se3 3.4892(14) 6_446 ?
Ba0A Se4 3.2582(19) . ?
Ba0A Se5 3.2588(11) 2_545 ?
Ba0A Se5 3.2587(11) 5_545 ?
Ba0A Se7 3.3495(19) 2_545 ?
Ba0A Se7 3.6166(19) 2_544 ?
In3 Ba1 4.07(3) 1_554 ?
In3 Se3 2.49(3) 1_556 ?
In3 Se4 2.57(3) . ?
In3 Se5 2.52(3) . ?
In3 Se6 2.49(3) . ?
Zn3 Se3 2.48(5) 1_556 ?
Zn3 Se4 2.57(5) . ?
Zn3 Se5 2.53(5) . ?
Zn3 Se6 2.49(5) . ?
In4 Se1 2.607(17) . ?
In4 Se2 2.643(10) 1_556 ?
In4 Se5 2.502(6) . ?
In4 Se5 2.502(6) 6_445 ?
Zn4 Se1 2.72(3) . ?
Zn4 Se2 2.43(2) 1_556 ?
Zn4 Se5 2.561(11) 6_445 ?
Zn4 Se5 2.561(11) . ?
In5 Ba1 3.906(16) 1_554 ?
In5 Ba1 3.906(16) 6_444 ?
In5 Ba0A 4.09(3) 1_554 ?
In5 Se2 2.54(3) . ?
In5 Se3 2.471(13) 6_445 ?
In5 Se3 2.471(13) . ?
In5 Se4 2.418(18) . ?
Zn5 Ba1 3.92(3) 1_554 ?
Zn5 Ba1 3.92(3) 6_444 ?
Zn5 Ba0A 3.97(4) 1_554 ?
Zn5 Se2 2.56(5) . ?
Zn5 Se3 2.40(2) 6_445 ?
Zn5 Se3 2.40(2) . ?
Zn5 Se4 2.61(3) . ?
Se1 Ba0A 3.3595(10) 2 ?
Se1 Ba0A 3.3595(10) 4_455 ?
Se1 In4 2.607(17) 3_455 ?
Se1 Zn4 2.72(3) 3_455 ?
Se1 In1 2.716(3) . ?
Se2 Ba1 3.2815(7) 1_554 ?
Se2 Ba1 3.2813(7) 6_444 ?
Se2 In4 2.643(10) 1_554 ?
Se2 Zn4 2.43(2) 1_554 ?
Se3 Ba1 3.4490(13) 1_554 ?
Se3 Ba1 3.2982(13) 2_545 ?
Se3 Ba0A 3.4892(14) 1_554 ?
Se3 In3 2.49(3) 1_554 ?
Se3 Zn3 2.48(5) 1_554 ?
Se4 In3 2.57(3) 6_445 ?
Se4 Zn3 2.57(5) 6_445 ?
Se5 Ba1 3.5012(15) 1_554 ?
Se5 Ba0A 3.2587(11) 4_455 ?
Se6 Ba1 3.2618(13) 2_545 ?
Se6 Ba1 3.4496(13) 1_554 ?
Se6 In2 2.5855(11) . ?
Se7 Ba1 3.5488(8) 1_554 ?
Se7 Ba1 3.5488(8) 8_454 ?
Se7 Ba0A 3.3495(19) 4_455 ?
Se7 Ba0A 3.6166(19) 4_454 ?
Se7 In1 2.5318(16) . ?
In1 Se7 2.5318(16) 3_455 ?
In2 Se6 2.5855(11) 3_445 ?
In2 Se6 2.5855(11) 4_455 ?
In2 Se6 2.5855(11) 2_545 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
In3 Ba1 Ba0A 82.2(4) 1_556 4_456 ?
In5 Ba1 Ba0A 116.8(3) 1_556 4_456 ?
In5 Ba1 In3 61.0(5) 1_556 1_556 ?
In5 Ba1 Zn5 3.0(7) 1_556 1_556 ?
Zn5 Ba1 Ba0A 119.0(5) 1_556 4_456 ?
Zn5 Ba1 In3 63.8(6) 1_556 1_556 ?
Se2 Ba1 Ba0A 86.77(3) 1_556 4_456 ?
Se2 Ba1 In3 79.3(4) 1_556 1_556 ?
Se2 Ba1 In5 40.3(4) 1_556 1_556 ?
Se2 Ba1 Zn5 40.4(6) 1_556 1_556 ?
Se2 Ba1 Se3 135.81(4) 1_556 4_455 ?
Se2 Ba1 Se3 76.19(3) 1_556 1_556 ?
Se2 Ba1 Se5 74.79(4) 1_556 1_556 ?
Se2 Ba1 Se5 72.76(4) 1_556 . ?
Se2 Ba1 Se6 111.76(4) 1_556 1_556 ?
Se2 Ba1 Se7 69.69(4) 1_556 1_556 ?
Se3 Ba1 Ba0A 49.08(3) 4_455 4_456 ?
Se3 Ba1 Ba0A 151.90(3) 1_556 4_456 ?
Se3 Ba1 In3 72.8(4) 1_556 1_556 ?
Se3 Ba1 In3 91.1(4) 4_455 1_556 ?
Se3 Ba1 In5 38.6(3) 1_556 1_556 ?
Se3 Ba1 In5 151.7(2) 4_455 1_556 ?
Se3 Ba1 Zn5 154.6(5) 4_455 1_556 ?
Se3 Ba1 Zn5 37.3(6) 1_556 1_556 ?
Se3 Ba1 Se3 141.76(4) 4_455 1_556 ?
Se3 Ba1 Se5 72.19(3) 1_556 . ?
Se3 Ba1 Se5 129.51(3) 4_455 . ?
Se3 Ba1 Se5 71.67(3) 4_455 1_556 ?
Se3 Ba1 Se5 108.12(3) 1_556 1_556 ?
Se3 Ba1 Se6 80.95(3) 4_455 1_556 ?
Se3 Ba1 Se6 65.02(3) 1_556 1_556 ?
Se3 Ba1 Se7 78.41(3) 4_455 1_556 ?
Se3 Ba1 Se7 139.76(4) 1_556 1_556 ?
Se5 Ba1 Ba0A 124.05(3) . 4_456 ?
Se5 Ba1 Ba0A 44.92(2) 1_556 4_456 ?
Se5 Ba1 In3 38.0(4) 1_556 1_556 ?
Se5 Ba1 In3 139.3(4) . 1_556 ?
Se5 Ba1 In5 82.3(2) 1_556 1_556 ?
Se5 Ba1 In5 78.7(3) . 1_556 ?
Se5 Ba1 Zn5 85.2(4) 1_556 1_556 ?
Se5 Ba1 Zn5 75.8(5) . 1_556 ?
Se5 Ba1 Se5 146.41(4) 1_556 . ?
Se5 Ba1 Se7 77.75(3) . 1_556 ?
Se5 Ba1 Se7 83.14(3) 1_556 1_556 ?
Se6 Ba1 Ba0A 102.30(3) 1_556 4_456 ?
Se6 Ba1 Ba0A 115.75(3) 4_455 4_456 ?
Se6 Ba1 In3 117.3(4) 4_455 1_556 ?
Se6 Ba1 In3 37.6(4) 1_556 1_556 ?
Se6 Ba1 In5 126.3(3) 4_455 1_556 ?
Se6 Ba1 In5 79.0(3) 1_556 1_556 ?
Se6 Ba1 Zn5 80.8(6) 1_556 1_556 ?
Se6 Ba1 Zn5 124.6(5) 4_455 1_556 ?
Se6 Ba1 Se2 152.57(4) 4_455 1_556 ?
Se6 Ba1 Se3 68.83(3) 4_455 4_455 ?
Se6 Ba1 Se3 87.74(3) 4_455 1_556 ?
Se6 Ba1 Se5 132.04(3) 4_455 1_556 ?
Se6 Ba1 Se5 81.27(3) 4_455 . ?
Se6 Ba1 Se5 67.80(3) 1_556 1_556 ?
Se6 Ba1 Se5 133.61(3) 1_556 . ?
Se6 Ba1 Se6 80.02(4) 4_455 1_556 ?
Se6 Ba1 Se7 148.47(4) 1_556 1_556 ?
Se6 Ba1 Se7 113.66(4) 4_455 1_556 ?
Se7 Ba1 Ba0A 46.33(3) 1_556 4_456 ?
Se7 Ba1 In3 119.3(4) 1_556 1_556 ?
Se7 Ba1 In5 109.9(4) 1_556 1_556 ?
Se7 Ba1 Zn5 109.7(6) 1_556 1_556 ?
In3 Ba0A In3 64.6(8) . 6_445 ?
In3 Ba0A In5 58.0(5) . 1_556 ?
In3 Ba0A In5 58.0(5) 6_445 1_556 ?
Zn5 Ba0A In3 56.1(6) 1_556 . ?
Zn5 Ba0A In3 56.1(6) 1_556 6_445 ?
Zn5 Ba0A In5 2.4(9) 1_556 1_556 ?
Se1 Ba0A In3 143.2(4) 2_545 . ?
Se1 Ba0A In3 143.2(4) 2_545 6_445 ?
Se1 Ba0A In5 147.4(3) 2_545 1_556 ?
Se1 Ba0A Zn5 149.9(6) 2_545 1_556 ?
Se1 Ba0A Se3 135.66(3) 2_545 1_556 ?
Se1 Ba0A Se3 135.66(3) 2_545 6_446 ?
Se1 Ba0A Se7 71.99(5) 2_545 2_544 ?
Se3 Ba0A In3 81.0(4) 1_556 6_445 ?
Se3 Ba0A In3 81.0(4) 6_446 . ?
Se3 Ba0A In3 37.4(4) 6_446 6_445 ?
Se3 Ba0A In3 37.4(4) 1_556 . ?
Se3 Ba0A In5 37.02(5) 1_556 1_556 ?
Se3 Ba0A In5 37.02(5) 6_446 1_556 ?
Se3 Ba0A Zn5 36.77(5) 1_556 1_556 ?
Se3 Ba0A Zn5 36.77(5) 6_446 1_556 ?
Se3 Ba0A Se3 73.30(4) 1_556 6_446 ?
Se3 Ba0A Se7 124.53(3) 1_556 2_544 ?
Se3 Ba0A Se7 124.53(3) 6_446 2_544 ?
Se4 Ba0A In3 39.1(4) . . ?
Se4 Ba0A In3 39.1(4) . 6_445 ?
Se4 Ba0A In5 74.4(3) . 1_556 ?
Se4 Ba0A Zn5 72.0(5) . 1_556 ?
Se4 Ba0A Se1 138.13(6) . 2_545 ?
Se4 Ba0A Se3 73.14(3) . 1_556 ?
Se4 Ba0A Se3 73.14(3) . 6_446 ?
Se4 Ba0A Se5 101.02(3) . 2_545 ?
Se4 Ba0A Se5 101.02(3) . 5_545 ?
Se4 Ba0A Se7 144.54(5) . 2_545 ?
Se4 Ba0A Se7 66.14(4) . 2_544 ?
Se5 Ba0A In3 74.6(4) 5_545 6_445 ?
Se5 Ba0A In3 138.0(4) 2_545 6_445 ?
Se5 Ba0A In3 74.6(4) 2_545 . ?
Se5 Ba0A In3 138.0(4) 5_545 . ?
Se5 Ba0A In5 108.25(4) 2_545 1_556 ?
Se5 Ba0A In5 108.25(4) 5_545 1_556 ?
Se5 Ba0A Zn5 108.51(6) 5_545 1_556 ?
Se5 Ba0A Zn5 108.51(7) 2_545 1_556 ?
Se5 Ba0A Se1 71.11(3) 5_545 2_545 ?
Se5 Ba0A Se1 71.11(3) 2_545 2_545 ?
Se5 Ba0A Se3 72.29(3) 5_545 6_446 ?
Se5 Ba0A Se3 72.29(3) 2_545 1_556 ?
Se5 Ba0A Se3 145.26(4) 5_545 1_556 ?
Se5 Ba0A Se3 145.26(4) 2_545 6_446 ?
Se5 Ba0A Se5 141.19(5) 5_545 2_545 ?
Se5 Ba0A Se7 90.12(3) 2_545 2_545 ?
Se5 Ba0A Se7 90.12(3) 5_545 2_545 ?
Se5 Ba0A Se7 80.14(3) 5_545 2_544 ?
Se5 Ba0A Se7 80.14(3) 2_545 2_544 ?
Se7 Ba0A In3 89.5(4) 2_544 . ?
Se7 Ba0A In3 116.0(4) 2_545 . ?
Se7 Ba0A In3 89.5(4) 2_544 6_445 ?
Se7 Ba0A In3 116.0(4) 2_545 6_445 ?
Se7 Ba0A In5 70.1(3) 2_545 1_556 ?
Se7 Ba0A In5 140.6(3) 2_544 1_556 ?
Se7 Ba0A Zn5 72.5(5) 2_545 1_556 ?
Se7 Ba0A Zn5 138.2(6) 2_544 1_556 ?
Se7 Ba0A Se1 77.33(5) 2_545 2_545 ?
Se7 Ba0A Se3 78.59(3) 2_545 1_556 ?
Se7 Ba0A Se3 78.59(3) 2_545 6_446 ?
Se7 Ba0A Se7 149.33(6) 2_545 2_544 ?
Ba1 In3 Ba0A 138.7(8) 1_554 . ?
Se3 In3 Ba1 162.4(11) 1_556 1_554 ?
Se3 In3 Ba0A 58.4(6) 1_556 . ?
Se3 In3 Se4 105.4(10) 1_556 . ?
Se3 In3 Se5 110.0(11) 1_556 . ?
Se3 In3 Se6 117.3(11) 1_556 . ?
Se4 In3 Ba1 91.7(7) . 1_554 ?
Se4 In3 Ba0A 53.0(5) . . ?
Se5 In3 Ba1 58.7(5) . 1_554 ?
Se5 In3 Ba0A 146.9(10) . . ?
Se5 In3 Se4 111.0(11) . . ?
Se6 In3 Ba1 57.5(5) . 1_554 ?
Se6 In3 Ba0A 111.6(9) . . ?
Se6 In3 Se4 112.0(11) . . ?
Se6 In3 Se5 101.3(10) . . ?
Se3 Zn3 Se4 105.6(17) 1_556 . ?
Se3 Zn3 Se5 110.0(18) 1_556 . ?
Se3 Zn3 Se6 117.7(19) 1_556 . ?
Se5 Zn3 Se4 110.6(17) . . ?
Se6 Zn3 Se4 111.9(18) . . ?
Se6 Zn3 Se5 101.0(16) . . ?
Se1 In4 Se2 121.7(7) . 1_556 ?
Se5 In4 Se1 97.8(3) . . ?
Se5 In4 Se1 97.8(3) 6_445 . ?
Se5 In4 Se2 103.3(3) 6_445 1_556 ?
Se5 In4 Se2 103.3(3) . 1_556 ?
Se5 In4 Se5 135.4(7) 6_445 . ?
Se2 Zn4 Se1 125.7(12) 1_556 . ?
Se2 Zn4 Se5 108.0(5) 1_556 6_445 ?
Se2 Zn4 Se5 108.0(5) 1_556 . ?
Se5 Zn4 Se1 93.5(6) . . ?
Se5 Zn4 Se1 93.5(6) 6_445 . ?
Se5 Zn4 Se5 129.3(11) 6_445 . ?
Ba1 In5 Ba1 113.0(7) 6_444 1_554 ?
Ba1 In5 Ba0A 117.7(3) 6_444 1_554 ?
Ba1 In5 Ba0A 117.7(3) 1_554 1_554 ?
Se2 In5 Ba1 56.5(4) . 6_444 ?
Se2 In5 Ba1 56.5(4) . 1_554 ?
Se2 In5 Ba0A 145.7(6) . 1_554 ?
Se3 In5 Ba1 156.2(8) . 6_444 ?
Se3 In5 Ba1 60.6(3) 6_445 6_444 ?
Se3 In5 Ba1 156.2(8) 6_445 1_554 ?
Se3 In5 Ba1 60.6(3) . 1_554 ?
Se3 In5 Ba0A 58.2(5) 6_445 1_554 ?
Se3 In5 Ba0A 58.2(5) . 1_554 ?
Se3 In5 Se2 111.9(7) 6_445 . ?
Se3 In5 Se2 111.9(7) . . ?
Se3 In5 Se3 114.9(9) . 6_445 ?
Se4 In5 Ba1 98.3(4) . 6_444 ?
Se4 In5 Ba1 98.3(4) . 1_554 ?
Se4 In5 Ba0A 107.3(9) . 1_554 ?
Se4 In5 Se2 107.0(8) . . ?
Se4 In5 Se3 105.2(7) . 6_445 ?
Se4 In5 Se3 105.2(7) . . ?
Ba1 Zn5 Ba1 112.5(12) 6_444 1_554 ?
Ba1 Zn5 Ba0A 120.3(5) 6_444 1_554 ?
Ba1 Zn5 Ba0A 120.3(5) 1_554 1_554 ?
Se2 Zn5 Ba1 56.3(6) . 1_554 ?
Se2 Zn5 Ba1 56.3(6) . 6_444 ?
Se2 Zn5 Ba0A 152.7(12) . 1_554 ?
Se2 Zn5 Se4 101.0(13) . . ?
Se3 Zn5 Ba1 60.7(5) 6_445 6_444 ?
Se3 Zn5 Ba1 162.8(15) 6_445 1_554 ?
Se3 Zn5 Ba1 162.8(15) . 6_444 ?
Se3 Zn5 Ba1 60.7(5) . 1_554 ?
Se3 Zn5 Ba0A 60.6(9) . 1_554 ?
Se3 Zn5 Ba0A 60.6(9) 6_445 1_554 ?
Se3 Zn5 Se2 114.0(12) 6_445 . ?
Se3 Zn5 Se2 114.0(12) . . ?
Se3 Zn5 Se3 120.6(18) . 6_445 ?
Se3 Zn5 Se4 101.6(11) . . ?
Se3 Zn5 Se4 101.6(11) 6_445 . ?
Se4 Zn5 Ba1 94.6(7) . 1_554 ?
Se4 Zn5 Ba1 94.6(7) . 6_444 ?
Se4 Zn5 Ba0A 106.3(15) . 1_554 ?
Ba0A Se1 Ba0A 173.45(8) 2 4_455 ?
In4 Se1 Ba0A 91.057(19) . 2 ?
In4 Se1 Ba0A 91.055(19) 3_455 2 ?
In4 Se1 Ba0A 91.056(19) . 4_455 ?
In4 Se1 Ba0A 91.058(19) 3_455 4_455 ?
In4 Se1 In4 142.3(6) . 3_455 ?
In4 Se1 Zn4 3.9(8) . . ?
In4 Se1 Zn4 3.9(8) 3_455 3_455 ?
In4 Se1 Zn4 138.4(3) 3_455 . ?
In4 Se1 Zn4 138.4(3) . 3_455 ?
In4 Se1 In1 108.8(3) 3_455 . ?
In4 Se1 In1 108.8(3) . . ?
Zn4 Se1 Ba0A 91.27(3) 3_455 2 ?
Zn4 Se1 Ba0A 91.26(3) . 4_455 ?
Zn4 Se1 Ba0A 91.27(3) . 2 ?
Zn4 Se1 Ba0A 91.26(3) 3_455 4_455 ?
Zn4 Se1 Zn4 134.5(10) 3_455 . ?
In1 Se1 Ba0A 86.73(4) . 2 ?
In1 Se1 Ba0A 86.73(4) . 4_455 ?
In1 Se1 Zn4 112.7(5) . . ?
In1 Se1 Zn4 112.7(5) . 3_455 ?
Ba1 Se2 Ba1 166.13(6) 6_444 1_554 ?
In4 Se2 Ba1 92.56(6) 1_554 6_444 ?
In4 Se2 Ba1 92.55(6) 1_554 1_554 ?
Zn4 Se2 Ba1 92.57(9) 1_554 1_554 ?
Zn4 Se2 Ba1 92.56(9) 1_554 6_444 ?
Zn4 Se2 In4 0.1(14) 1_554 1_554 ?
Zn4 Se2 In5 101.5(9) 1_554 . ?
Zn4 Se2 Zn5 96.9(10) 1_554 . ?
In5 Se2 Ba1 83.18(3) . 1_554 ?
In5 Se2 Ba1 83.18(3) . 6_444 ?
In5 Se2 In4 101.4(6) . 1_554 ?
In5 Se2 Zn5 4.6(11) . . ?
Zn5 Se2 Ba1 83.30(4) . 1_554 ?
Zn5 Se2 Ba1 83.30(4) . 6_444 ?
Zn5 Se2 In4 96.8(8) . 1_554 ?
Ba1 Se3 Ba1 111.89(4) 2_545 1_554 ?
Ba1 Se3 Ba0A 85.34(3) 2_545 1_554 ?
Ba1 Se3 Ba0A 161.05(4) 1_554 1_554 ?
In3 Se3 Ba1 88.1(7) 1_554 1_554 ?
In3 Se3 Ba1 136.4(7) 1_554 2_545 ?
In3 Se3 Ba0A 84.2(7) 1_554 1_554 ?
Zn3 Se3 Ba1 136.2(11) 1_554 2_545 ?
Zn3 Se3 Ba1 88.2(11) 1_554 1_554 ?
Zn3 Se3 Ba0A 84.1(11) 1_554 1_554 ?
Zn3 Se3 In3 0.2(19) 1_554 1_554 ?
In5 Se3 Ba1 80.7(6) . 1_554 ?
In5 Se3 Ba1 115.3(5) . 2_545 ?
In5 Se3 Ba0A 84.8(5) . 1_554 ?
In5 Se3 In3 105.8(8) . 1_554 ?
In5 Se3 Zn3 105.9(12) . 1_554 ?
Zn5 Se3 Ba1 82.0(10) . 1_554 ?
Zn5 Se3 Ba1 118.9(10) . 2_545 ?
Zn5 Se3 Ba0A 82.6(10) . 1_554 ?
Zn5 Se3 In3 101.5(11) . 1_554 ?
Zn5 Se3 Zn3 101.7(14) . 1_554 ?
Zn5 Se3 In5 4.5(11) . . ?
In3 Se4 Ba0A 87.9(6) 6_445 . ?
In3 Se4 Ba0A 87.9(6) . . ?
In3 Se4 In3 115.8(13) 6_445 . ?
In3 Se4 Zn3 0.3(17) . . ?
In3 Se4 Zn3 0.3(17) 6_445 6_445 ?
In3 Se4 Zn3 115.8(4) . 6_445 ?
In3 Se4 Zn3 115.8(4) 6_445 . ?
In3 Se4 Zn5 109.2(8) 6_445 . ?
In3 Se4 Zn5 109.2(8) . . ?
Zn3 Se4 Ba0A 87.6(10) . . ?
Zn3 Se4 Ba0A 87.6(10) 6_445 . ?
Zn3 Se4 Zn3 116(2) 6_445 . ?
Zn3 Se4 Zn5 109.5(11) 6_445 . ?
Zn3 Se4 Zn5 109.5(11) . . ?
In5 Se4 Ba0A 147.1(7) . . ?
In5 Se4 In3 108.6(7) . 6_445 ?
In5 Se4 In3 108.6(7) . . ?
In5 Se4 Zn3 108.8(11) . . ?
In5 Se4 Zn3 108.8(11) . 6_445 ?
In5 Se4 Zn5 1.4(18) . . ?
Zn5 Se4 Ba0A 145.7(11) . . ?
Ba1 Se5 Ba1 146.41(4) 1_554 . ?
Ba0A Se5 Ba1 85.74(3) 4_455 1_554 ?
Ba0A Se5 Ba1 95.98(4) 4_455 . ?
In3 Se5 Ba1 86.1(6) . . ?
In3 Se5 Ba1 83.4(6) . 1_554 ?
In3 Se5 Ba0A 163.1(7) . 4_455 ?
In3 Se5 Zn3 0.2(18) . . ?
In3 Se5 Zn4 100.3(10) . . ?
Zn3 Se5 Ba1 83.5(10) . 1_554 ?
Zn3 Se5 Ba1 85.9(11) . . ?
Zn3 Se5 Ba0A 163.1(11) . 4_455 ?
Zn3 Se5 Zn4 100.3(13) . . ?
In4 Se5 Ba1 123.7(2) . 1_554 ?
In4 Se5 Ba1 89.7(2) . . ?
In4 Se5 Ba0A 95.4(4) . 4_455 ?
In4 Se5 In3 101.5(8) . . ?
In4 Se5 Zn3 101.5(12) . . ?
In4 Se5 Zn4 4.7(7) . . ?
Zn4 Se5 Ba1 128.2(4) . 1_554 ?
Zn4 Se5 Ba1 85.1(4) . . ?
Zn4 Se5 Ba0A 96.6(7) . 4_455 ?
Ba1 Se6 Ba1 112.79(3) 2_545 1_554 ?
In3 Se6 Ba1 104.6(7) . 2_545 ?
In3 Se6 Ba1 84.9(6) . 1_554 ?
In3 Se6 In2 104.2(7) . . ?
Zn3 Se6 Ba1 104.4(11) . 2_545 ?
Zn3 Se6 Ba1 85.2(11) . 1_554 ?
Zn3 Se6 In3 0.3(18) . . ?
Zn3 Se6 In2 104.0(11) . . ?
In2 Se6 Ba1 124.21(4) . 1_554 ?
In2 Se6 Ba1 117.34(4) . 2_545 ?
Ba1 Se7 Ba1 152.57(5) 1_554 8_454 ?
Ba1 Se7 Ba0A 89.33(3) 8_454 4_454 ?
Ba1 Se7 Ba0A 89.33(3) 1_554 4_454 ?
Ba0A Se7 Ba1 83.64(3) 4_455 1_554 ?
Ba0A Se7 Ba1 83.65(3) 4_455 8_454 ?
Ba0A Se7 Ba0A 149.33(6) 4_455 4_454 ?
In1 Se7 Ba1 102.10(3) . 1_554 ?
In1 Se7 Ba1 102.10(3) . 8_454 ?
In1 Se7 Ba0A 89.98(6) . 4_455 ?
In1 Se7 Ba0A 120.70(7) . 4_454 ?
Se7 In1 Se1 105.96(6) . . ?
Se7 In1 Se1 105.96(6) 3_455 . ?
Se7 In1 Se7 148.07(11) . 3_455 ?
Se6 In2 Se6 115.55(3) 3_445 2_545 ?
Se6 In2 Se6 115.55(3) 3_445 4_455 ?
Se6 In2 Se6 115.55(3) . 2_545 ?
Se6 In2 Se6 97.89(5) 2_545 4_455 ?
Se6 In2 Se6 97.89(5) 3_445 . ?
Se6 In2 Se6 115.55(3) . 4_455 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
Ba1 In3 Se4 Ba0A -156.6(4) 1_554 . . . ?
Ba1 In3 Se4 In3 116.8(9) 1_554 . . 6_445 ?
Ba1 In3 Se4 Zn3 -149(100) 1_554 . . . ?
Ba1 In3 Se4 Zn3 117.1(11) 1_554 . . 6_445 ?
Ba1 In3 Se4 In5 -5.6(9) 1_554 . . . ?
Ba1 In3 Se4 Zn5 -6.9(12) 1_554 . . . ?
Ba1 In3 Se5 Ba1 148.05(13) 1_554 . . . ?
Ba1 In3 Se5 Ba0A 50(2) 1_554 . . 4_455 ?
Ba1 In3 Se5 Zn3 145(100) 1_554 . . . ?
Ba1 In3 Se5 In4 -123.1(3) 1_554 . . . ?
Ba1 In3 Se5 Zn4 -127.7(4) 1_554 . . . ?
Ba1 In3 Se6 Ba1 112.24(16) 1_554 . . 2_545 ?
Ba1 In3 Se6 Zn3 175(100) 1_554 . . . ?
Ba1 In3 Se6 In2 -124.03(15) 1_554 . . . ?
Ba1 In5 Se2 Ba1 177.51(11) 1_554 . . 6_444 ?
Ba1 In5 Se2 Ba1 -177.51(11) 6_444 . . 1_554 ?
Ba1 In5 Se2 In4 -91.24(5) 1_554 . . 1_554 ?
Ba1 In5 Se2 In4 91.25(5) 6_444 . . 1_554 ?
Ba1 In5 Se2 Zn4 -91.24(5) 1_554 . . 1_554 ?
Ba1 In5 Se2 Zn4 91.24(5) 6_444 . . 1_554 ?
Ba1 In5 Se2 Zn5 -91.24(3) 1_554 . . . ?
Ba1 In5 Se2 Zn5 91.24(9) 6_444 . . . ?
Ba1 In5 Se3 Ba1 -81(2) 6_444 . . 1_554 ?
Ba1 In5 Se3 Ba1 -109.9(3) 1_554 . . 2_545 ?
Ba1 In5 Se3 Ba1 169.6(19) 6_444 . . 2_545 ?
Ba1 In5 Se3 Ba0A 167.76(12) 1_554 . . 1_554 ?
Ba1 In5 Se3 Ba0A 87(2) 6_444 . . 1_554 ?
Ba1 In5 Se3 In3 85.3(7) 1_554 . . 1_554 ?
Ba1 In5 Se3 In3 5(2) 6_444 . . 1_554 ?
Ba1 In5 Se3 Zn3 85.5(12) 1_554 . . 1_554 ?
Ba1 In5 Se3 Zn3 5(3) 6_444 . . 1_554 ?
Ba1 In5 Se3 Zn5 26(20) 6_444 . . . ?
Ba1 In5 Se3 Zn5 106(22) 1_554 . . . ?
Ba1 In5 Se4 Ba0A 122.6(4) 1_554 . . . ?
Ba1 In5 Se4 Ba0A -122.6(4) 6_444 . . . ?
Ba1 In5 Se4 In3 -5.9(9) 6_444 . . 6_445 ?
Ba1 In5 Se4 In3 -120.8(7) 1_554 . . 6_445 ?
Ba1 In5 Se4 In3 5.9(9) 1_554 . . . ?
Ba1 In5 Se4 In3 120.8(7) 6_444 . . . ?
Ba1 In5 Se4 Zn3 121.0(11) 6_444 . . . ?
Ba1 In5 Se4 Zn3 6.1(13) 1_554 . . . ?
Ba1 In5 Se4 Zn3 -121.0(11) 1_554 . . 6_445 ?
Ba1 In5 Se4 Zn3 -6.1(13) 6_444 . . 6_445 ?
Ba1 In5 Se4 Zn5 -122.6(6) 6_444 . . . ?
Ba1 In5 Se4 Zn5 122.6(3) 1_554 . . . ?
Ba1 Zn5 Se2 Ba1 176.42(17) 1_554 . . 6_444 ?
Ba1 Zn5 Se2 Ba1 -176.42(17) 6_444 . . 1_554 ?
Ba1 Zn5 Se2 In4 -91.79(9) 1_554 . . 1_554 ?
Ba1 Zn5 Se2 In4 91.79(9) 6_444 . . 1_554 ?
Ba1 Zn5 Se2 Zn4 91.79(9) 6_444 . . 1_554 ?
Ba1 Zn5 Se2 Zn4 -91.79(9) 1_554 . . 1_554 ?
Ba1 Zn5 Se2 In5 -88.21(11) 6_444 . . . ?
Ba1 Zn5 Se2 In5 88.21(7) 1_554 . . . ?
Ba1 Zn5 Se3 Ba1 179(4) 6_444 . . 2_545 ?
Ba1 Zn5 Se3 Ba1 -71(5) 6_444 . . 1_554 ?
Ba1 Zn5 Se3 Ba1 -110.6(5) 1_554 . . 2_545 ?
Ba1 Zn5 Se3 Ba0A 98(5) 6_444 . . 1_554 ?
Ba1 Zn5 Se3 Ba0A 168.9(2) 1_554 . . 1_554 ?
Ba1 Zn5 Se3 In3 86.4(7) 1_554 . . 1_554 ?
Ba1 Zn5 Se3 In3 16(5) 6_444 . . 1_554 ?
Ba1 Zn5 Se3 Zn3 16(5) 6_444 . . 1_554 ?
Ba1 Zn5 Se3 Zn3 86.5(12) 1_554 . . 1_554 ?
Ba1 Zn5 Se3 In5 -144(26) 6_444 . . . ?
Ba1 Zn5 Se3 In5 -73(22) 1_554 . . . ?
Ba1 Zn5 Se4 Ba0A 123.5(7) 1_554 . . . ?
Ba1 Zn5 Se4 Ba0A -123.5(7) 6_444 . . . ?
Ba1 Zn5 Se4 In3 -120.3(8) 1_554 . . 6_445 ?
Ba1 Zn5 Se4 In3 -7.2(12) 6_444 . . 6_445 ?
Ba1 Zn5 Se4 In3 120.3(8) 6_444 . . . ?
Ba1 Zn5 Se4 In3 7.2(12) 1_554 . . . ?
Ba1 Zn5 Se4 Zn3 -7.5(15) 6_444 . . 6_445 ?
Ba1 Zn5 Se4 Zn3 -120.5(12) 1_554 . . 6_445 ?
Ba1 Zn5 Se4 Zn3 7.5(15) 1_554 . . . ?
Ba1 Zn5 Se4 Zn3 120.5(12) 6_444 . . . ?
Ba1 Zn5 Se4 In5 56.5(7) 6_444 . . . ?
Ba1 Zn5 Se4 In5 -56.5(6) 1_554 . . . ?
Ba1 Se6 In2 Se6 157.61(5) 2_545 . . 4_455 ?
Ba1 Se6 In2 Se6 -164.32(5) 1_554 . . 2_545 ?
Ba1 Se6 In2 Se6 -50.91(3) 1_554 . . 4_455 ?
Ba1 Se6 In2 Se6 72.38(4) 1_554 . . 3_445 ?
Ba1 Se6 In2 Se6 -79.09(4) 2_545 . . 3_445 ?
Ba1 Se6 In2 Se6 44.20(3) 2_545 . . 2_545 ?
Ba1 Se7 In1 Se1 -83.50(4) 1_554 . . . ?
Ba1 Se7 In1 Se1 83.50(4) 8_454 . . . ?
Ba1 Se7 In1 Se7 96.51(4) 1_554 . . 3_455 ?
Ba1 Se7 In1 Se7 -96.50(4) 8_454 . . 3_455 ?
Ba0A Ba1 Se5 Ba1 -121.81(6) 4_456 . . 1_554 ?
Ba0A Ba1 Se5 Ba0A -30.52(4) 4_456 . . 4_455 ?
Ba0A Ba1 Se5 In3 166.4(7) 4_456 . . . ?
Ba0A Ba1 Se5 Zn3 166.4(11) 4_456 . . . ?
Ba0A Ba1 Se5 In4 64.8(4) 4_456 . . . ?
Ba0A Ba1 Se5 Zn4 65.7(7) 4_456 . . . ?
Ba0A In3 Se4 In3 -86.6(10) . . . 6_445 ?
Ba0A In3 Se4 Zn3 -86.3(8) . . . 6_445 ?
Ba0A In3 Se4 Zn3 8(100) . . . . ?
Ba0A In3 Se4 In5 150.9(7) . . . . ?
Ba0A In3 Se4 Zn5 149.6(10) . . . . ?
Ba0A In3 Se5 Ba1 -79.4(17) . . . . ?
Ba0A In3 Se5 Ba1 132.5(18) . . . 1_554 ?
Ba0A In3 Se5 Ba0A -177.1(4) . . . 4_455 ?
Ba0A In3 Se5 Zn3 -82(100) . . . . ?
Ba0A In3 Se5 In4 9.4(19) . . . . ?
Ba0A In3 Se5 Zn4 4.8(19) . . . . ?
Ba0A In3 Se6 Ba1 -134.9(7) . . . 1_554 ?
Ba0A In3 Se6 Ba1 -22.6(9) . . . 2_545 ?
Ba0A In3 Se6 Zn3 41(100) . . . . ?
Ba0A In3 Se6 In2 101.1(7) . . . . ?
Ba0A In5 Se2 Ba1 91.24(6) 1_554 . . 1_554 ?
Ba0A In5 Se2 Ba1 -91.24(6) 1_554 . . 6_444 ?
Ba0A In5 Se2 In4 0.002(4) 1_554 . . 1_554 ?
Ba0A In5 Se2 Zn4 0.000(4) 1_554 . . 1_554 ?
Ba0A In5 Se2 Zn5 0.00(3) 1_554 . . . ?
Ba0A In5 Se3 Ba1 82.3(2) 1_554 . . 2_545 ?
Ba0A In5 Se3 Ba1 -167.76(12) 1_554 . . 1_554 ?
Ba0A In5 Se3 In3 -82.4(7) 1_554 . . 1_554 ?
Ba0A In5 Se3 Zn3 -82.3(12) 1_554 . . 1_554 ?
Ba0A In5 Se3 Zn5 -62(22) 1_554 . . . ?
Ba0A In5 Se4 Ba0A -0.001(2) 1_554 . . . ?
Ba0A In5 Se4 In3 116.6(7) 1_554 . . 6_445 ?
Ba0A In5 Se4 In3 -116.6(7) 1_554 . . . ?
Ba0A In5 Se4 Zn3 116.5(11) 1_554 . . 6_445 ?
Ba0A In5 Se4 Zn3 -116.5(11) 1_554 . . . ?
Ba0A In5 Se4 Zn5 0.00(15) 1_554 . . . ?
Ba0A Zn5 Se2 Ba1 91.79(9) 1_554 . . 1_554 ?
Ba0A Zn5 Se2 Ba1 -91.79(9) 1_554 . . 6_444 ?
Ba0A Zn5 Se2 In4 0.002(9) 1_554 . . 1_554 ?
Ba0A Zn5 Se2 Zn4 0.000(9) 1_554 . . 1_554 ?
Ba0A Zn5 Se2 In5 180.00(2) 1_554 . . . ?
Ba0A Zn5 Se3 Ba1 -168.9(2) 1_554 . . 1_554 ?
Ba0A Zn5 Se3 Ba1 80.5(5) 1_554 . . 2_545 ?
Ba0A Zn5 Se3 In3 -82.5(7) 1_554 . . 1_554 ?
Ba0A Zn5 Se3 Zn3 -82.4(12) 1_554 . . 1_554 ?
Ba0A Zn5 Se3 In5 118(22) 1_554 . . . ?
Ba0A Zn5 Se4 Ba0A 0.000(3) 1_554 . . . ?
Ba0A Zn5 Se4 In3 -116.2(7) 1_554 . . . ?
Ba0A Zn5 Se4 In3 116.2(7) 1_554 . . 6_445 ?
Ba0A Zn5 Se4 Zn3 -116.0(12) 1_554 . . . ?
Ba0A Zn5 Se4 Zn3 116.0(12) 1_554 . . 6_445 ?
Ba0A Zn5 Se4 In5 180(3) 1_554 . . . ?
Ba0A Se1 In1 Se7 0.0 2 . . 3_455 ?
Ba0A Se1 In1 Se7 180.0 4_455 . . 3_455 ?
Ba0A Se1 In1 Se7 0.0 4_455 . . . ?
Ba0A Se1 In1 Se7 180.0 2 . . . ?
Ba0A Se7 In1 Se1 180.0 4_454 . . . ?
Ba0A Se7 In1 Se1 0.0 4_455 . . . ?
Ba0A Se7 In1 Se7 180.0 4_455 . . 3_455 ?
Ba0A Se7 In1 Se7 0.0 4_454 . . 3_455 ?
In3 Ba1 Se5 Ba1 115.7(6) 1_556 . . 1_554 ?
In3 Ba1 Se5 Ba0A -153.0(6) 1_556 . . 4_455 ?
In3 Ba1 Se5 In3 43.9(5) 1_556 . . . ?
In3 Ba1 Se5 Zn3 43.9(16) 1_556 . . . ?
In3 Ba1 Se5 In4 -57.6(7) 1_556 . . . ?
In3 Ba1 Se5 Zn4 -56.8(9) 1_556 . . . ?
In3 Ba0A In3 Ba1 75.9(12) 6_445 . . 1_554 ?
In3 Ba0A In3 Se3 -109.6(5) 6_445 . . 1_556 ?
In3 Ba0A In3 Se4 38.9(7) 6_445 . . . ?
In3 Ba0A In3 Se5 -32(2) 6_445 . . . ?
In3 Ba0A In3 Se6 140.8(7) 6_445 . . . ?
In3 Ba0A Se4 In3 115.9(13) . . . 6_445 ?
In3 Ba0A Se4 In3 -115.9(13) 6_445 . . . ?
In3 Ba0A Se4 Zn3 0.0(17) . . . . ?
In3 Ba0A Se4 Zn3 116.0(4) . . . 6_445 ?
In3 Ba0A Se4 Zn3 -116.0(4) 6_445 . . . ?
In3 Ba0A Se4 Zn3 0.0(17) 6_445 . . 6_445 ?
In3 Ba0A Se4 In5 122.0(6) 6_445 . . . ?
In3 Ba0A Se4 In5 -122.0(6) . . . . ?
In3 Ba0A Se4 Zn5 122.0(6) 6_445 . . . ?
In3 Ba0A Se4 Zn5 -122.0(6) . . . . ?
In3 Se6 In2 Se6 165.9(7) . . . 3_445 ?
In3 Se6 In2 Se6 42.6(7) . . . 4_455 ?
In3 Se6 In2 Se6 -70.8(7) . . . 2_545 ?
Zn3 Se6 In2 Se6 42.9(11) . . . 4_455 ?
Zn3 Se6 In2 Se6 166.2(11) . . . 3_445 ?
Zn3 Se6 In2 Se6 -70.5(11) . . . 2_545 ?
In4 Se1 In1 Se7 90.0 . . . . ?
In4 Se1 In1 Se7 -90.0 . . . 3_455 ?
In4 Se1 In1 Se7 -90.0 3_455 . . . ?
In4 Se1 In1 Se7 90.0 3_455 . . 3_455 ?
Zn4 Se1 In1 Se7 -90.0 . . . 3_455 ?
Zn4 Se1 In1 Se7 90.0 . . . . ?
Zn4 Se1 In1 Se7 -90.0 3_455 . . . ?
Zn4 Se1 In1 Se7 90.0 3_455 . . 3_455 ?
In5 Ba1 Se5 Ba1 123.3(4) 1_556 . . 1_554 ?
In5 Ba1 Se5 Ba0A -145.4(4) 1_556 . . 4_455 ?
In5 Ba1 Se5 In3 51.5(7) 1_556 . . . ?
In5 Ba1 Se5 Zn3 51.5(11) 1_556 . . . ?
In5 Ba1 Se5 In4 -50.0(6) 1_556 . . . ?
In5 Ba1 Se5 Zn4 -49.2(8) 1_556 . . . ?
In5 Ba0A In3 Ba1 142.6(13) 1_556 . . 1_554 ?
In5 Ba0A In3 Se3 -42.9(4) 1_556 . . 1_556 ?
In5 Ba0A In3 Se4 105.6(7) 1_556 . . . ?
In5 Ba0A In3 Se5 35.0(16) 1_556 . . . ?
In5 Ba0A In3 Se6 -152.5(11) 1_556 . . . ?
In5 Ba0A Se4 In3 -58.0(6) 1_556 . . . ?
In5 Ba0A Se4 In3 58.0(6) 1_556 . . 6_445 ?
In5 Ba0A Se4 Zn3 58.0(10) 1_556 . . 6_445 ?
In5 Ba0A Se4 Zn3 -58.0(10) 1_556 . . . ?
In5 Ba0A Se4 In5 180.000(3) 1_556 . . . ?
In5 Ba0A Se4 Zn5 179.999(5) 1_556 . . . ?
Zn5 Ba1 Se5 Ba1 122.6(6) 1_556 . . 1_554 ?
Zn5 Ba1 Se5 Ba0A -146.1(6) 1_556 . . 4_455 ?
Zn5 Ba1 Se5 In3 50.7(9) 1_556 . . . ?
Zn5 Ba1 Se5 Zn3 50.7(12) 1_556 . . . ?
Zn5 Ba1 Se5 In4 -50.8(7) 1_556 . . . ?
Zn5 Ba1 Se5 Zn4 -50.0(9) 1_556 . . . ?
Zn5 Ba0A In3 Ba1 140.8(14) 1_556 . . 1_554 ?
Zn5 Ba0A In3 Se3 -44.8(6) 1_556 . . 1_556 ?
Zn5 Ba0A In3 Se4 103.7(8) 1_556 . . . ?
Zn5 Ba0A In3 Se5 33.2(16) 1_556 . . . ?
Zn5 Ba0A In3 Se6 -154.4(12) 1_556 . . . ?
Zn5 Ba0A Se4 In3 -58.0(6) 1_556 . . . ?
Zn5 Ba0A Se4 In3 58.0(6) 1_556 . . 6_445 ?
Zn5 Ba0A Se4 Zn3 -58.0(10) 1_556 . . . ?
Zn5 Ba0A Se4 Zn3 58.0(10) 1_556 . . 6_445 ?
Zn5 Ba0A Se4 In5 179.999(4) 1_556 . . . ?
Zn5 Ba0A Se4 Zn5 179.999(5) 1_556 . . . ?
Se1 Ba0A In3 Ba1 -72.0(14) 2_545 . . 1_554 ?
Se1 Ba0A In3 Se3 102.5(7) 2_545 . . 1_556 ?
Se1 Ba0A In3 Se4 -109.0(6) 2_545 . . . ?
Se1 Ba0A In3 Se5 -179.5(13) 2_545 . . . ?
Se1 Ba0A In3 Se6 -7.1(14) 2_545 . . . ?
Se1 Ba0A Se4 In3 -122.0(6) 2_545 . . 6_445 ?
Se1 Ba0A Se4 In3 122.0(6) 2_545 . . . ?
Se1 Ba0A Se4 Zn3 122.0(10) 2_545 . . . ?
Se1 Ba0A Se4 Zn3 -122.0(10) 2_545 . . 6_445 ?
Se1 Ba0A Se4 In5 0.001(4) 2_545 . . . ?
Se1 Ba0A Se4 Zn5 0.001(6) 2_545 . . . ?
Se1 In4 Se5 Ba1 -114.5(3) . . . . ?
Se1 In4 Se5 Ba1 69.9(5) . . . 1_554 ?
Se1 In4 Se5 Ba0A -18.5(3) . . . 4_455 ?
Se1 In4 Se5 In3 159.6(7) . . . . ?
Se1 In4 Se5 Zn3 159.8(11) . . . . ?
Se1 In4 Se5 Zn4 -124(14) . . . . ?
Se1 Zn4 Se5 Ba1 66.8(10) . . . 1_554 ?
Se1 Zn4 Se5 Ba1 -118.4(5) . . . . ?
Se1 Zn4 Se5 Ba0A -23.0(5) . . . 4_455 ?
Se1 Zn4 Se5 In3 156.5(8) . . . . ?
Se1 Zn4 Se5 Zn3 156.7(12) . . . . ?
Se1 Zn4 Se5 In4 52(13) . . . . ?
Se2 Ba1 Se5 Ba1 164.50(7) 1_556 . . 1_554 ?
Se2 Ba1 Se5 Ba0A -104.21(4) 1_556 . . 4_455 ?
Se2 Ba1 Se5 In3 92.7(7) 1_556 . . . ?
Se2 Ba1 Se5 Zn3 92.7(11) 1_556 . . . ?
Se2 Ba1 Se5 In4 -8.8(4) 1_556 . . . ?
Se2 Ba1 Se5 Zn4 -8.0(7) 1_556 . . . ?
Se2 In4 Se1 Ba0A 93.10(4) 1_556 . . 2 ?
Se2 In4 Se1 Ba0A -93.10(4) 1_556 . . 4_455 ?
Se2 In4 Se1 In4 0.000(1) 1_556 . . 3_455 ?
Se2 In4 Se1 Zn4 -0.001(2) 1_556 . . . ?
Se2 In4 Se1 Zn4 0.0 1_556 . . 3_455 ?
Se2 In4 Se1 In1 180.0 1_556 . . . ?
Se2 In4 Se5 Ba1 10.8(5) 1_556 . . . ?
Se2 In4 Se5 Ba1 -164.8(2) 1_556 . . 1_554 ?
Se2 In4 Se5 Ba0A 106.8(5) 1_556 . . 4_455 ?
Se2 In4 Se5 In3 -75.1(8) 1_556 . . . ?
Se2 In4 Se5 Zn3 -75.0(12) 1_556 . . . ?
Se2 In4 Se5 Zn4 1(13) 1_556 . . . ?
Se2 Zn4 Se1 Ba0A 93.02(4) 1_556 . . 2 ?
Se2 Zn4 Se1 Ba0A -93.02(4) 1_556 . . 4_455 ?
Se2 Zn4 Se1 In4 0.0 1_556 . . 3_455 ?
Se2 Zn4 Se1 In4 180.00(5) 1_556 . . . ?
Se2 Zn4 Se1 Zn4 -0.003(2) 1_556 . . 3_455 ?
Se2 Zn4 Se1 In1 180.0 1_556 . . . ?
Se2 Zn4 Se5 Ba1 10.9(9) 1_556 . . . ?
Se2 Zn4 Se5 Ba1 -163.8(5) 1_556 . . 1_554 ?
Se2 Zn4 Se5 Ba0A 106.4(10) 1_556 . . 4_455 ?
Se2 Zn4 Se5 In3 -74.2(12) 1_556 . . . ?
Se2 Zn4 Se5 Zn3 -74.0(15) 1_556 . . . ?
Se2 Zn4 Se5 In4 -179(100) 1_556 . . . ?
Se2 In5 Se3 Ba1 -24.8(4) . . . 1_554 ?
Se2 In5 Se3 Ba1 -134.7(5) . . . 2_545 ?
Se2 In5 Se3 Ba0A 142.9(5) . . . 1_554 ?
Se2 In5 Se3 In3 60.5(9) . . . 1_554 ?
Se2 In5 Se3 Zn3 60.6(13) . . . 1_554 ?
Se2 In5 Se3 Zn5 81(22) . . . . ?
Se2 In5 Se4 Ba0A 180.000(1) . . . . ?
Se2 In5 Se4 In3 63.4(7) . . . . ?
Se2 In5 Se4 In3 -63.4(7) . . . 6_445 ?
Se2 In5 Se4 Zn3 -63.5(11) . . . 6_445 ?
Se2 In5 Se4 Zn3 63.5(11) . . . . ?
Se2 In5 Se4 Zn5 180(3) . . . . ?
Se2 Zn5 Se3 Ba1 -129.6(10) . . . 2_545 ?
Se2 Zn5 Se3 Ba1 -18.9(9) . . . 1_554 ?
Se2 Zn5 Se3 Ba0A 149.9(11) . . . 1_554 ?
Se2 Zn5 Se3 In3 67.5(13) . . . 1_554 ?
Se2 Zn5 Se3 Zn3 67.6(16) . . . 1_554 ?
Se2 Zn5 Se3 In5 -92(22) . . . . ?
Se2 Zn5 Se4 Ba0A 180.000(2) . . . . ?
Se2 Zn5 Se4 In3 -63.8(7) . . . 6_445 ?
Se2 Zn5 Se4 In3 63.8(7) . . . . ?
Se2 Zn5 Se4 Zn3 -64.0(12) . . . 6_445 ?
Se2 Zn5 Se4 Zn3 64.0(12) . . . . ?
Se2 Zn5 Se4 In5 0.00(10) . . . . ?
Se3 Ba1 Se5 Ba1 83.87(7) 1_556 . . 1_554 ?
Se3 Ba1 Se5 Ba1 -59.68(9) 4_455 . . 1_554 ?
Se3 Ba1 Se5 Ba0A 175.16(4) 1_556 . . 4_455 ?
Se3 Ba1 Se5 Ba0A 31.61(5) 4_455 . . 4_455 ?
Se3 Ba1 Se5 In3 -131.5(7) 4_455 . . . ?
Se3 Ba1 Se5 In3 12.0(7) 1_556 . . . ?
Se3 Ba1 Se5 Zn3 12.1(11) 1_556 . . . ?
Se3 Ba1 Se5 Zn3 -131.5(11) 4_455 . . . ?
Se3 Ba1 Se5 In4 -89.5(4) 1_556 . . . ?
Se3 Ba1 Se5 In4 127.0(4) 4_455 . . . ?
Se3 Ba1 Se5 Zn4 127.8(7) 4_455 . . . ?
Se3 Ba1 Se5 Zn4 -88.7(7) 1_556 . . . ?
Se3 Ba0A In3 Ba1 111.3(11) 6_446 . . 1_554 ?
Se3 Ba0A In3 Ba1 -174.5(16) 1_556 . . 1_554 ?
Se3 Ba0A In3 Se3 -74.2(5) 6_446 . . 1_556 ?
Se3 Ba0A In3 Se4 148.5(10) 1_556 . . . ?
Se3 Ba0A In3 Se4 74.3(5) 6_446 . . . ?
Se3 Ba0A In3 Se5 3.7(17) 6_446 . . . ?
Se3 Ba0A In3 Se5 78.0(17) 1_556 . . . ?
Se3 Ba0A In3 Se6 176.2(9) 6_446 . . . ?
Se3 Ba0A In3 Se6 -109.6(12) 1_556 . . . ?
Se3 Ba0A Se4 In3 -96.6(6) 6_446 . . . ?
Se3 Ba0A Se4 In3 96.6(6) 1_556 . . 6_445 ?
Se3 Ba0A Se4 In3 19.4(6) 6_446 . . 6_445 ?
Se3 Ba0A Se4 In3 -19.4(6) 1_556 . . . ?
Se3 Ba0A Se4 Zn3 -96.6(10) 6_446 . . . ?
Se3 Ba0A Se4 Zn3 19.4(10) 6_446 . . 6_445 ?
Se3 Ba0A Se4 Zn3 96.6(10) 1_556 . . 6_445 ?
Se3 Ba0A Se4 Zn3 -19.4(10) 1_556 . . . ?
Se3 Ba0A Se4 In5 -141.41(2) 1_556 . . . ?
Se3 Ba0A Se4 In5 141.41(2) 6_446 . . . ?
Se3 Ba0A Se4 Zn5 141.41(2) 6_446 . . . ?
Se3 Ba0A Se4 Zn5 -141.41(2) 1_556 . . . ?
Se3 In3 Se4 Ba0A 27.5(8) 1_556 . . . ?
Se3 In3 Se4 In3 -59.1(16) 1_556 . . 6_445 ?
Se3 In3 Se4 Zn3 36(100) 1_556 . . . ?
Se3 In3 Se4 Zn3 -58.8(8) 1_556 . . 6_445 ?
Se3 In3 Se4 In5 178.4(9) 1_556 . . . ?
Se3 In3 Se4 Zn5 177.1(12) 1_556 . . . ?
Se3 In3 Se5 Ba1 -165.1(10) 1_556 . . 1_554 ?
Se3 In3 Se5 Ba1 -17.0(9) 1_556 . . . ?
Se3 In3 Se5 Ba0A -114.7(19) 1_556 . . 4_455 ?
Se3 In3 Se5 Zn3 -20(100) 1_556 . . . ?
Se3 In3 Se5 In4 71.9(10) 1_556 . . . ?
Se3 In3 Se5 Zn4 67.2(11) 1_556 . . . ?
Se3 In3 Se6 Ba1 160.6(12) 1_556 . . 1_554 ?
Se3 In3 Se6 Ba1 -87.2(11) 1_556 . . 2_545 ?
Se3 In3 Se6 Zn3 -24(100) 1_556 . . . ?
Se3 In3 Se6 In2 36.6(12) 1_556 . . . ?
Se3 Zn3 Se4 Ba0A 27.7(14) 1_556 . . . ?
Se3 Zn3 Se4 In3 -144(100) 1_556 . . . ?
Se3 Zn3 Se4 In3 -58.8(13) 1_556 . . 6_445 ?
Se3 Zn3 Se4 Zn3 -58(3) 1_556 . . 6_445 ?
Se3 Zn3 Se4 In5 178.6(13) 1_556 . . . ?
Se3 Zn3 Se4 Zn5 177.3(14) 1_556 . . . ?
Se3 Zn3 Se5 Ba1 -165.2(17) 1_556 . . 1_554 ?
Se3 Zn3 Se5 Ba1 -17.1(15) 1_556 . . . ?
Se3 Zn3 Se5 Ba0A -114(3) 1_556 . . 4_455 ?
Se3 Zn3 Se5 In3 160(100) 1_556 . . . ?
Se3 Zn3 Se5 In4 71.7(17) 1_556 . . . ?
Se3 Zn3 Se5 Zn4 67.1(17) 1_556 . . . ?
Se3 Zn3 Se6 Ba1 160.4(19) 1_556 . . 1_554 ?
Se3 Zn3 Se6 Ba1 -87.3(19) 1_556 . . 2_545 ?
Se3 Zn3 Se6 In3 156(100) 1_556 . . . ?
Se3 Zn3 Se6 In2 36(2) 1_556 . . . ?
Se3 In5 Se2 Ba1 -26.0(5) 6_445 . . 6_444 ?
Se3 In5 Se2 Ba1 156.5(6) 6_445 . . 1_554 ?
Se3 In5 Se2 Ba1 -156.5(6) . . . 6_444 ?
Se3 In5 Se2 Ba1 26.0(5) . . . 1_554 ?
Se3 In5 Se2 In4 -65.2(5) . . . 1_554 ?
Se3 In5 Se2 In4 65.2(5) 6_445 . . 1_554 ?
Se3 In5 Se2 Zn4 65.2(5) 6_445 . . 1_554 ?
Se3 In5 Se2 Zn4 -65.2(5) . . . 1_554 ?
Se3 In5 Se2 Zn5 -65.2(5) . . . . ?
Se3 In5 Se2 Zn5 65.2(5) 6_445 . . . ?
Se3 In5 Se3 Ba1 -153.7(10) 6_445 . . 1_554 ?
Se3 In5 Se3 Ba1 96.4(8) 6_445 . . 2_545 ?
Se3 In5 Se3 Ba0A 14.0(9) 6_445 . . 1_554 ?
Se3 In5 Se3 In3 -68.4(13) 6_445 . . 1_554 ?
Se3 In5 Se3 Zn3 -68.3(15) 6_445 . . 1_554 ?
Se3 In5 Se3 Zn5 -48(21) 6_445 . . . ?
Se3 In5 Se4 Ba0A -60.9(8) 6_445 . . . ?
Se3 In5 Se4 Ba0A 60.9(8) . . . . ?
Se3 In5 Se4 In3 55.8(12) 6_445 . . 6_445 ?
Se3 In5 Se4 In3 177.5(9) . . . 6_445 ?
Se3 In5 Se4 In3 -55.8(12) . . . . ?
Se3 In5 Se4 In3 -177.5(9) 6_445 . . . ?
Se3 In5 Se4 Zn3 177.3(13) . . . 6_445 ?
Se3 In5 Se4 Zn3 -55.6(15) . . . . ?
Se3 In5 Se4 Zn3 -177.3(13) 6_445 . . . ?
Se3 In5 Se4 Zn3 55.6(15) 6_445 . . 6_445 ?
Se3 In5 Se4 Zn5 -60.9(9) 6_445 . . . ?
Se3 In5 Se4 Zn5 60.9(6) . . . . ?
Se3 Zn5 Se2 Ba1 -19.9(10) 6_445 . . 6_444 ?
Se3 Zn5 Se2 Ba1 163.7(12) 6_445 . . 1_554 ?
Se3 Zn5 Se2 Ba1 -163.7(12) . . . 6_444 ?
Se3 Zn5 Se2 Ba1 19.9(10) . . . 1_554 ?
Se3 Zn5 Se2 In4 71.9(11) 6_445 . . 1_554 ?
Se3 Zn5 Se2 In4 -71.9(11) . . . 1_554 ?
Se3 Zn5 Se2 Zn4 -71.9(11) . . . 1_554 ?
Se3 Zn5 Se2 Zn4 71.9(11) 6_445 . . 1_554 ?
Se3 Zn5 Se2 In5 -108.1(11) 6_445 . . . ?
Se3 Zn5 Se2 In5 108.1(11) . . . . ?
Se3 Zn5 Se3 Ba1 -160.1(18) 6_445 . . 1_554 ?
Se3 Zn5 Se3 Ba1 89.2(16) 6_445 . . 2_545 ?
Se3 Zn5 Se3 Ba0A 8.7(16) 6_445 . . 1_554 ?
Se3 Zn5 Se3 In3 -74(2) 6_445 . . 1_554 ?
Se3 Zn5 Se3 Zn3 -74(2) 6_445 . . 1_554 ?
Se3 Zn5 Se3 In5 127(23) 6_445 . . . ?
Se3 Zn5 Se4 Ba0A 62.5(12) . . . . ?
Se3 Zn5 Se4 Ba0A -62.5(12) 6_445 . . . ?
Se3 Zn5 Se4 In3 53.7(17) 6_445 . . 6_445 ?
Se3 Zn5 Se4 In3 -178.7(11) 6_445 . . . ?
Se3 Zn5 Se4 In3 -53.7(17) . . . . ?
Se3 Zn5 Se4 In3 178.7(12) . . . 6_445 ?
Se3 Zn5 Se4 Zn3 -178.5(14) 6_445 . . . ?
Se3 Zn5 Se4 Zn3 178.5(14) . . . 6_445 ?
Se3 Zn5 Se4 Zn3 -54(2) . . . . ?
Se3 Zn5 Se4 Zn3 54(2) 6_445 . . 6_445 ?
Se3 Zn5 Se4 In5 -117.5(12) . . . . ?
Se3 Zn5 Se4 In5 117.5(13) 6_445 . . . ?
Se4 Ba0A In3 Ba1 37.0(7) . . . 1_554 ?
Se4 Ba0A In3 Se3 -148.5(10) . . . 1_556 ?
Se4 Ba0A In3 Se5 -70.5(17) . . . . ?
Se4 Ba0A In3 Se6 101.9(11) . . . . ?
Se4 In3 Se5 Ba1 -133.2(9) . . . . ?
Se4 In3 Se5 Ba1 78.7(9) . . . 1_554 ?
Se4 In3 Se5 Ba0A 129.1(17) . . . 4_455 ?
Se4 In3 Se5 Zn3 -136(100) . . . . ?
Se4 In3 Se5 In4 -44.3(10) . . . . ?
Se4 In3 Se5 Zn4 -49.0(11) . . . . ?
Se4 In3 Se6 Ba1 34.8(11) . . . 2_545 ?
Se4 In3 Se6 Ba1 -77.4(9) . . . 1_554 ?
Se4 In3 Se6 Zn3 98(100) . . . . ?
Se4 In3 Se6 In2 158.5(8) . . . . ?
Se4 Zn3 Se5 Ba1 78.5(15) . . . 1_554 ?
Se4 Zn3 Se5 Ba1 -133.4(15) . . . . ?
Se4 Zn3 Se5 Ba0A 130(3) . . . 4_455 ?
Se4 Zn3 Se5 In3 44(100) . . . . ?
Se4 Zn3 Se5 In4 -44.6(16) . . . . ?
Se4 Zn3 Se5 Zn4 -49.2(17) . . . . ?
Se4 Zn3 Se6 Ba1 35.4(18) . . . 2_545 ?
Se4 Zn3 Se6 Ba1 -77.0(15) . . . 1_554 ?
Se4 Zn3 Se6 In3 -82(100) . . . . ?
Se4 Zn3 Se6 In2 158.9(13) . . . . ?
Se4 In5 Se2 Ba1 -88.76(5) . . . 1_554 ?
Se4 In5 Se2 Ba1 88.76(5) . . . 6_444 ?
Se4 In5 Se2 In4 180.001(2) . . . 1_554 ?
Se4 In5 Se2 Zn4 179.999(3) . . . 1_554 ?
Se4 In5 Se2 Zn5 180.00(4) . . . . ?
Se4 In5 Se3 Ba1 -18.9(10) . . . 2_545 ?
Se4 In5 Se3 Ba1 91.0(7) . . . 1_554 ?
Se4 In5 Se3 Ba0A -101.2(8) . . . 1_554 ?
Se4 In5 Se3 In3 176.4(9) . . . 1_554 ?
Se4 In5 Se3 Zn3 176.5(13) . . . 1_554 ?
Se4 In5 Se3 Zn5 -163(23) . . . . ?
Se4 Zn5 Se2 Ba1 -88.21(9) . . . 1_554 ?
Se4 Zn5 Se2 Ba1 88.21(9) . . . 6_444 ?
Se4 Zn5 Se2 In4 180.001(2) . . . 1_554 ?
Se4 Zn5 Se2 Zn4 179.999(3) . . . 1_554 ?
Se4 Zn5 Se2 In5 0.00(2) . . . . ?
Se4 Zn5 Se3 Ba1 88.8(11) . . . 1_554 ?
Se4 Zn5 Se3 Ba1 -21.8(16) . . . 2_545 ?
Se4 Zn5 Se3 Ba0A -102.3(12) . . . 1_554 ?
Se4 Zn5 Se3 In3 175.2(12) . . . 1_554 ?
Se4 Zn5 Se3 Zn3 175.3(15) . . . 1_554 ?
Se4 Zn5 Se3 In5 16(21) . . . . ?
Se5 Ba1 Se5 Ba1 180.0 1_556 . . 1_554 ?
Se5 Ba1 Se5 Ba0A -88.71(7) 1_556 . . 4_455 ?
Se5 Ba1 Se5 In3 108.2(7) 1_556 . . . ?
Se5 Ba1 Se5 Zn3 108.2(11) 1_556 . . . ?
Se5 Ba1 Se5 In4 6.7(4) 1_556 . . . ?
Se5 Ba1 Se5 Zn4 7.5(7) 1_556 . . . ?
Se5 Ba0A In3 Ba1 60.8(13) 5_545 . . 1_554 ?
Se5 Ba0A In3 Ba1 -93.7(11) 2_545 . . 1_554 ?
Se5 Ba0A In3 Se3 80.8(5) 2_545 . . 1_556 ?
Se5 Ba0A In3 Se3 -124.7(5) 5_545 . . 1_556 ?
Se5 Ba0A In3 Se4 23.8(9) 5_545 . . . ?
Se5 Ba0A In3 Se4 -130.7(6) 2_545 . . . ?
Se5 Ba0A In3 Se5 -47(2) 5_545 . . . ?
Se5 Ba0A In3 Se5 158.7(19) 2_545 . . . ?
Se5 Ba0A In3 Se6 125.7(7) 5_545 . . . ?
Se5 Ba0A In3 Se6 -28.8(8) 2_545 . . . ?
Se5 Ba0A Se4 In3 164.0(6) 2_545 . . 6_445 ?
Se5 Ba0A Se4 In3 -164.0(6) 5_545 . . . ?
Se5 Ba0A Se4 In3 48.1(6) 2_545 . . . ?
Se5 Ba0A Se4 In3 -48.1(6) 5_545 . . 6_445 ?
Se5 Ba0A Se4 Zn3 164.1(10) 2_545 . . 6_445 ?
Se5 Ba0A Se4 Zn3 -164.1(10) 5_545 . . . ?
Se5 Ba0A Se4 Zn3 48.1(10) 2_545 . . . ?
Se5 Ba0A Se4 Zn3 -48.1(10) 5_545 . . 6_445 ?
Se5 Ba0A Se4 In5 -73.93(3) 2_545 . . . ?
Se5 Ba0A Se4 In5 73.92(3) 5_545 . . . ?
Se5 Ba0A Se4 Zn5 -73.93(3) 2_545 . . . ?
Se5 Ba0A Se4 Zn5 73.92(3) 5_545 . . . ?
Se5 In3 Se4 Ba0A 146.5(9) . . . . ?
Se5 In3 Se4 In3 59.9(16) . . . 6_445 ?
Se5 In3 Se4 Zn3 60.2(9) . . . 6_445 ?
Se5 In3 Se4 Zn3 155(100) . . . . ?
Se5 In3 Se4 In5 -62.6(12) . . . . ?
Se5 In3 Se4 Zn5 -63.9(14) . . . . ?
Se5 In3 Se6 Ba1 153.2(7) . . . 2_545 ?
Se5 In3 Se6 Ba1 40.9(8) . . . 1_554 ?
Se5 In3 Se6 Zn3 -144(100) . . . . ?
Se5 In3 Se6 In2 -83.1(8) . . . . ?
Se5 Zn3 Se4 Ba0A 146.7(15) . . . . ?
Se5 Zn3 Se4 In3 -25(100) . . . . ?
Se5 Zn3 Se4 In3 60.2(14) . . . 6_445 ?
Se5 Zn3 Se4 Zn3 61(3) . . . 6_445 ?
Se5 Zn3 Se4 In5 -62.4(18) . . . . ?
Se5 Zn3 Se4 Zn5 -64(2) . . . . ?
Se5 Zn3 Se6 Ba1 153.0(11) . . . 2_545 ?
Se5 Zn3 Se6 Ba1 40.7(12) . . . 1_554 ?
Se5 Zn3 Se6 In3 36(100) . . . . ?
Se5 Zn3 Se6 In2 -83.4(13) . . . . ?
Se5 In4 Se1 Ba0A 17.9(3) . . . 4_455 ?
Se5 In4 Se1 Ba0A 155.9(3) 6_445 . . 4_455 ?
Se5 In4 Se1 Ba0A -17.9(3) 6_445 . . 2 ?
Se5 In4 Se1 Ba0A -155.9(3) . . . 2 ?
Se5 In4 Se1 In4 111.0(3) . . . 3_455 ?
Se5 In4 Se1 In4 -111.0(3) 6_445 . . 3_455 ?
Se5 In4 Se1 Zn4 -111.0(3) 6_445 . . . ?
Se5 In4 Se1 Zn4 111.0(3) . . . . ?
Se5 In4 Se1 Zn4 111.0(3) . . . 3_455 ?
Se5 In4 Se1 Zn4 -111.0(3) 6_445 . . 3_455 ?
Se5 In4 Se1 In1 -69.0(3) . . . . ?
Se5 In4 Se1 In1 69.0(3) 6_445 . . . ?
Se5 In4 Se5 Ba1 -39.5(11) 6_445 . . 1_554 ?
Se5 In4 Se5 Ba1 136.1(8) 6_445 . . . ?
Se5 In4 Se5 Ba0A -128.0(8) 6_445 . . 4_455 ?
Se5 In4 Se5 In3 50.1(11) 6_445 . . . ?
Se5 In4 Se5 Zn3 50.3(13) 6_445 . . . ?
Se5 In4 Se5 Zn4 126(14) 6_445 . . . ?
Se5 Zn4 Se1 Ba0A 22.1(5) . . . 4_455 ?
Se5 Zn4 Se1 Ba0A -22.1(5) 6_445 . . 2 ?
Se5 Zn4 Se1 Ba0A 151.9(5) 6_445 . . 4_455 ?
Se5 Zn4 Se1 Ba0A -151.9(5) . . . 2 ?
Se5 Zn4 Se1 In4 -115.1(5) 6_445 . . 3_455 ?
Se5 Zn4 Se1 In4 115.1(5) . . . 3_455 ?
Se5 Zn4 Se1 In4 64.9(5) 6_445 . . . ?
Se5 Zn4 Se1 In4 -64.9(5) . . . . ?
Se5 Zn4 Se1 Zn4 115.1(5) . . . 3_455 ?
Se5 Zn4 Se1 Zn4 -115.1(5) 6_445 . . 3_455 ?
Se5 Zn4 Se1 In1 -64.9(5) . . . . ?
Se5 Zn4 Se1 In1 64.9(5) 6_445 . . . ?
Se5 Zn4 Se5 Ba1 -30.5(19) 6_445 . . 1_554 ?
Se5 Zn4 Se5 Ba1 144.2(14) 6_445 . . . ?
Se5 Zn4 Se5 Ba0A -120.3(13) 6_445 . . 4_455 ?
Se5 Zn4 Se5 In3 59.1(15) 6_445 . . . ?
Se5 Zn4 Se5 Zn3 59.3(17) 6_445 . . . ?
Se5 Zn4 Se5 In4 -46(12) 6_445 . . . ?
Se6 Ba1 Se5 Ba1 -6.55(7) 4_455 . . 1_554 ?
Se6 Ba1 Se5 Ba1 60.59(9) 1_556 . . 1_554 ?
Se6 Ba1 Se5 Ba0A 151.88(4) 1_556 . . 4_455 ?
Se6 Ba1 Se5 Ba0A 84.74(4) 4_455 . . 4_455 ?
Se6 Ba1 Se5 In3 -11.2(7) 1_556 . . . ?
Se6 Ba1 Se5 In3 -78.4(7) 4_455 . . . ?
Se6 Ba1 Se5 Zn3 -11.2(11) 1_556 . . . ?
Se6 Ba1 Se5 Zn3 -78.4(11) 4_455 . . . ?
Se6 Ba1 Se5 In4 -179.9(4) 4_455 . . . ?
Se6 Ba1 Se5 In4 -112.8(4) 1_556 . . . ?
Se6 Ba1 Se5 Zn4 -179.1(7) 4_455 . . . ?
Se6 Ba1 Se5 Zn4 -111.9(7) 1_556 . . . ?
Se6 In3 Se4 Ba0A -101.1(10) . . . . ?
Se6 In3 Se4 In3 172.28(15) . . . 6_445 ?
Se6 In3 Se4 Zn3 172.6(18) . . . 6_445 ?
Se6 In3 Se4 Zn3 -93(100) . . . . ?
Se6 In3 Se4 In5 49.9(13) . . . . ?
Se6 In3 Se4 Zn5 48.5(15) . . . . ?
Se6 In3 Se5 Ba1 107.7(8) . . . . ?
Se6 In3 Se5 Ba1 -40.3(7) . . . 1_554 ?
Se6 In3 Se5 Ba0A 10(3) . . . 4_455 ?
Se6 In3 Se5 Zn3 105(100) . . . . ?
Se6 In3 Se5 In4 -163.4(7) . . . . ?
Se6 In3 Se5 Zn4 -168.0(8) . . . . ?
Se6 Zn3 Se4 Ba0A -101.6(16) . . . . ?
Se6 Zn3 Se4 In3 172.0(18) . . . 6_445 ?
Se6 Zn3 Se4 In3 86(100) . . . . ?
Se6 Zn3 Se4 Zn3 172.3(2) . . . 6_445 ?
Se6 Zn3 Se4 In5 49.3(19) . . . . ?
Se6 Zn3 Se4 Zn5 48(2) . . . . ?
Se6 Zn3 Se5 Ba1 108.0(13) . . . . ?
Se6 Zn3 Se5 Ba1 -40.1(12) . . . 1_554 ?
Se6 Zn3 Se5 Ba0A 11(5) . . . 4_455 ?
Se6 Zn3 Se5 In3 -75(100) . . . . ?
Se6 Zn3 Se5 In4 -163.2(11) . . . . ?
Se6 Zn3 Se5 Zn4 -167.8(12) . . . . ?
Se7 Ba1 Se5 Ba1 -123.22(7) 1_556 . . 1_554 ?
Se7 Ba1 Se5 Ba0A -31.94(3) 1_556 . . 4_455 ?
Se7 Ba1 Se5 In3 164.9(7) 1_556 . . . ?
Se7 Ba1 Se5 Zn3 165.0(11) 1_556 . . . ?
Se7 Ba1 Se5 In4 63.4(4) 1_556 . . . ?
Se7 Ba1 Se5 Zn4 64.2(7) 1_556 . . . ?
Se7 Ba0A In3 Ba1 -176.2(9) 2_545 . . 1_554 ?
Se7 Ba0A In3 Ba1 -13.8(11) 2_544 . . 1_554 ?
Se7 Ba0A In3 Se3 -1.7(7) 2_545 . . 1_556 ?
Se7 Ba0A In3 Se3 160.7(5) 2_544 . . 1_556 ?
Se7 Ba0A In3 Se4 146.8(3) 2_545 . . . ?
Se7 Ba0A In3 Se4 -50.8(5) 2_544 . . . ?
Se7 Ba0A In3 Se5 76.3(19) 2_545 . . . ?
Se7 Ba0A In3 Se5 -121.4(18) 2_544 . . . ?
Se7 Ba0A In3 Se6 51.1(9) 2_544 . . . ?
Se7 Ba0A In3 Se6 -111.3(8) 2_545 . . . ?
Se7 Ba0A Se4 In3 -58.0(6) 2_545 . . . ?
Se7 Ba0A Se4 In3 122.0(6) 2_544 . . . ?
Se7 Ba0A Se4 In3 -122.0(6) 2_544 . . 6_445 ?
Se7 Ba0A Se4 In3 58.0(6) 2_545 . . 6_445 ?
Se7 Ba0A Se4 Zn3 58.0(10) 2_545 . . 6_445 ?
Se7 Ba0A Se4 Zn3 -58.0(10) 2_545 . . . ?
Se7 Ba0A Se4 Zn3 -122.0(10) 2_544 . . 6_445 ?
Se7 Ba0A Se4 Zn3 122.0(10) 2_544 . . . ?
Se7 Ba0A Se4 In5 179.999(4) 2_545 . . . ?
Se7 Ba0A Se4 In5 0.001(4) 2_544 . . . ?
Se7 Ba0A Se4 Zn5 179.999(5) 2_545 . . . ?
Se7 Ba0A Se4 Zn5 0.001(6) 2_544 . . . ?
_olex2_submission_special_instructions 'No special instructions were received'
loop_
_twin_individual_id
_twin_individual_mass_fraction_refined
1 0.92(2)
2 0.08(2)

